Above room-temperature dielectric switching and semiconducting properties of a layered organic-inorganic hybrid compound: (C<sub>6</sub>H<sub>12</sub>N)<sub>2</sub>Pb(NO<sub>3</sub>)<sub>4</sub>.
Jiang, Jia-Ying; Xu, Qi; Ma, Jia-Jun; Gong, Zhi-Xin; Shi, Chao; Zhang, Yi; Dalton transactions (Cambridge, England : 2003) 49 (2020) 16860–16865; doi:10.1039/d0dt03206a

data_7705894
_publ_section_title
;
 Above room-temperature dielectric switching and semiconducting properties
 of a layered organic-inorganic hybrid compound:
 (C<sub>6</sub>H<sub>12</sub>N)<sub>2</sub>Pb(NO<sub>3</sub>)<sub>4</sub>.
;
_journal_issue                   46
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16860
_journal_page_last               16865
_journal_paper_doi               10.1039/d0dt03206a
_journal_volume                  49
_journal_year                    2020
_chemical_formula_moiety         'N4 O12 Pb, 2(C6 H12 N)'
_chemical_formula_sum            'C12 H24 N6 O12 Pb'
_chemical_formula_weight         651.57
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-10-22 deposited with the CCDC.	2020-10-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 91.584(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.9554(2)
_cell_length_b                   22.6284(6)
_cell_length_c                   13.8537(3)
_cell_measurement_reflns_used    8746
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.9660
_cell_measurement_theta_min      2.3180
_cell_volume                     2179.59(10)
_computing_data_collection       'CrysAlisPro 1.171.40.39a (Rigaku OD, 2019)'
_computing_molecular_graphics    'Diamond 3.2 (Brandenburg, 2014)'
_computing_publication_material  'Word 2018'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.836
_diffrn_measurement_device_type  Rigaku
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0242
_diffrn_reflns_av_unetI/netI     0.0323
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.836
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            17136
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.836
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.520
_diffrn_reflns_theta_min         1.724
_exptl_absorpt_coefficient_mu    7.811
_exptl_absorpt_correction_T_max  0.210
_exptl_absorpt_correction_T_min  0.110
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            clourless
_exptl_crystal_density_diffrn    1.986
_exptl_crystal_description       block
_exptl_crystal_F_000             1264
_exptl_crystal_size_max          0.345
_exptl_crystal_size_mid          0.276
_exptl_crystal_size_min          0.228
_refine_diff_density_max         0.751
_refine_diff_density_min         -1.058
_refine_diff_density_rms         0.086
_refine_ls_extinction_coef       0.00082(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.005
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     281
_refine_ls_number_reflns         6078
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.005
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0297
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0284P)^2^+0.5665P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0563
_refine_ls_wR_factor_ref         0.0597
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4756
_reflns_number_total             7271
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0dt03206a2.cif
_cod_data_source_block           LTP
_cod_original_cell_volume        2179.60(10)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               7705894
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.121
_shelx_estimated_absorpt_t_max   0.384
_shelx_res_checksum              14497